# chapter 6: diffusion

Post on 31-Dec-2015

55 views

Embed Size (px)

DESCRIPTION

Chapter 6: Diffusion. ISSUES TO ADDRESS. • How does diffusion occur?. • Why is it an important part of processing?. • How can the rate of diffusion be predicted for some simple cases?. • How does diffusion depend on structure and temperature?. Diffusion. - PowerPoint PPT PresentationTRANSCRIPT

Chapter 6: Diffusion

1ISSUES TO ADDRESS... How does diffusion occur? Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases? How does diffusion depend on structure and temperature?Chapter 6: DiffusionChapter 6 -12DiffusionDiffusion - Mass transport by atomic motion

MechanismsGases & Liquids random (Brownian) motionSolids vacancy diffusion or interstitial diffusionChapter 6 -23 Interdiffusion: In an alloy, atoms tend to migrate from regions of high conc. to regions of low conc.Initially

Adapted from Figs. 6.1 and 6.2, Callister & Rethwisch 4e.DiffusionAfter some time

Chapter 6 -34 Self-diffusion: In an elemental solid, atoms also migrate.Label some atomsDiffusionABCDAfter some timeABCDChapter 6 -45Diffusion MechanismsVacancy Diffusion: atoms exchange with vacancies applies to substitutional impurities atoms rate depends on: -- number of vacancies -- activation energy to exchange.increasing elapsed timeChapter 6 -56 Simulation of interdiffusion across an interface: Rate of substitutional diffusion depends on: -- vacancy concentration -- frequency of jumping(Courtesy P.M. Anderson)Diffusion Simulation

This slide contains an animation that requires Quicktime and a Cinepak decompressor. Click on the message or image below to activate the animation.Chapter 6 -67Diffusion MechanismsInterstitial diffusion smaller atoms can diffuse between atoms.More rapid than vacancy diffusionAdapted from Fig. 6.3 (b), Callister & Rethwisch 4e.

Chapter 6 -78Adapted from chapter-opening photograph, Chapter 6, Callister & Rethwisch 4e. (Courtesy ofSurface Division, Midland-Ross.)

Case Hardening: -- Diffuse carbon atoms into the host iron atoms at the surface. -- Example of interstitial diffusion is a case hardened gear. Result: The presence of C atoms makes iron (steel) harder. Processing Using DiffusionChapter 6 -89 Doping silicon with phosphorus for n-type semiconductors: Process:3. Result: Doped semiconductor regions.siliconProcessing Using Diffusion

magnified image of a computer chip 0.5 mm light regions: Si atoms light regions: Al atoms 2. Heat it.1. Deposit P rich layers on surface.siliconAdapted from Figure 12.27, Callister & Rethwisch 4e.Chapter 6 -910DiffusionHow do we quantify the amount or rate of diffusion?

J slope

M =massdiffusedtimeMeasured empiricallyMake thin film (membrane) of known cross-sectional areaImpose concentration gradientMeasure how fast atoms or molecules diffuse through the membraneChapter 6 -1011Steady-State Diffusion

Ficks first law of diffusionC1C2 xC1C2x1x2D diffusion coefficientRate of diffusion independent of timeFlux proportional to concentration gradient =

Chapter 6 -1112Example: Chemical Protective Clothing (CPC)Methylene chloride is a common ingredient of paint removers. Besides being an irritant, it also may be absorbed through skin. When using this paint remover, protective gloves should be worn.If butyl rubber gloves (0.04 cm thick) are used, what is the diffusive flux of methylene chloride through the glove?Data:diffusion coefficient in butyl rubber: D = 110 x10-8 cm2/ssurface concentrations: C2 = 0.02 g/cm3C1 = 0.44 g/cm3Chapter 6 -1213

Example (cont).

gloveC1C2skinpaintremoverx1x2 Solution assuming linear conc. gradientD = 110 x 10-8 cm2/s C2 = 0.02 g/cm3C1 = 0.44 g/cm3x2 x1 = 0.04 cmData:Chapter 6 -1314Diffusion and Temperature Diffusion coefficient increases with increasing TD=Doexp -QdRT= pre-exponential [m2/s]= diffusion coefficient [m2/s]= activation energy [J/mol or eV/atom] = gas constant [8.314 J/mol-K]= absolute temperature [K]DDoQdRTChapter 6 -1415Diffusion and TemperatureAdapted from Fig. 6.7, Callister & Rethwisch 4e. (Date for Fig. 6.7 taken from E.A. Brandes and G.B. Brook (Ed.) Smithells Metals Reference Book, 7th ed., Butterworth-Heinemann, Oxford, 1992.)D has exponential dependence on TDinterstitial >> DsubstitutionalC in a-FeC in g-FeAl in AlFe in a-FeFe in g-Fe1000 K/TD (m2/s)C in a-Fe C in g-Fe Al in AlFe in a-Fe Fe in g-Fe 0.51.01.510-2010-1410-8T(C)15001000600300Chapter 6 -1516Example: At 300C the diffusion coefficient and activation energy for Cu in Si are

D(300C) = 7.8 x 10-11 m2/sQd = 41.5 kJ/mol

What is the diffusion coefficient at 350C?

transform dataDTemp = Tln D1/TChapter 6 -1617Example (cont.)

T1 = 273 + 300 = 573 KT2 = 273 + 350 = 623 KD2 = 15.7 x 10-11 m2/sChapter 6 -1718Non-steady State DiffusionThe concentration of diffusing species is a function of both time and position C = C(x,t)In this case Ficks Second Law is used

Ficks Second LawChapter 6 -18In the non-steady state the concentration profile develops with time. VMSE: Screenshot of Diffusion Computations & Data Plots19

Chapter 6 -20Non-steady State DiffusionAdapted from Fig. 6.5, Callister & Rethwisch 4e. B.C. at t = 0, C = Co for 0 x at t > 0, C = CS for x = 0 (constant surface conc.) C = Co for x = Copper diffuses into a bar of aluminum.pre-existing conc., Co of copper atoms Surface conc., C of Cu atomsbars

CsChapter 6 -2021Solution: C(x,t) = Conc. at point x at time t erf (z) = error function

erf(z) values are given in Table 6.1CSCoC(x,t)

Adapted from Fig. 6.5, Callister & Rethwisch 4e. Chapter 6 -2122Non-steady State DiffusionSample Problem: An FCC iron-carbon alloy initially containing 0.20 wt% C is carburized at an elevated temperature and in an atmosphere that gives a surface carbon concentration constant at 1.0 wt%. If after 49.5 h the concentration of carbon is 0.35 wt% at a position 4.0 mm below the surface, determine the temperature at which the treatment was carried out.

Solution: use Eqn. 6.5

Chapter 6 -2223Solution (cont.):t = 49.5 h x = 4 x 10-3 mCx = 0.35 wt%Cs = 1.0 wt%Co = 0.20 wt%

erf(z) = 0.8125Chapter 6 -2324Solution (cont.):We must now determine from Table 6.1 the value of z for which the error function is 0.8125. An interpolation is necessary as followszerf(z)0.900.7970z0.81250.950.8209

z = 0.93Now solve for D

Chapter 6 -2425To solve for the temperature at which D has the above value, we use a rearranged form of Equation (6.9a);

from Table 6.2, for diffusion of C in FCC Fe Do = 2.3 x 10-5 m2/s Qd = 148,000 J/mol

Solution (cont.):T = 1300 K = 1027CChapter 6 -2526Example: Chemical Protective Clothing (CPC)Methylene chloride is a common ingredient of paint removers. Besides being an irritant, it also may be absorbed through skin. When using this paint remover, protective gloves should be worn.If butyl rubber gloves (0.04 cm thick) are used, what is the breakthrough time (tb), i.e., how long could the gloves be used before methylene chloride reaches the hand?Datadiffusion coefficient in butyl rubber: D = 110 x10-8 cm2/sChapter 6 -2627CPC Example (cont.)Time required for breakthrough ca. 4 mingloveC1C2skinpaintremoverx1x2 Solution assuming linear conc. gradient

Equation from online CPC Case Study 5 at the Student Companion Site for Callister & Rethwisch 4e (www.wiley.com/college/callister)

D = 110 x 10-8 cm2/s

Breakthrough time = tbChapter 6 -2728Diffusion FASTER for...

open crystal structures

materials w/secondary bonding

smaller diffusing atoms

lower density materialsDiffusion SLOWER for...

close-packed structures

materials w/covalent bonding

larger diffusing atoms

higher density materialsSummaryChapter 6 -2829Core Problems:Self-help Problems:ANNOUNCEMENTSReading:Chapter 6 -29